GEBERT AND R.J. , ~ C K E R R I A N N 136 ELIZABETH
Recently, Edwards and Pearsonl' have discussed important factors which contribute to nucleophilicity. Basicity and polarizability of the nucleophile play an important role. In the (CHB)zSOH22+substrate, nucleophilic attack a t either sulfur or oxygen should be correlated by a combination of basicity and polarizability in the nucleophile, because each center bears a positive charge and possesses an unshared pair of electrons. Since polarizability increases and basicity decreases in the series C1-, Br-, I-, the two factors cannot be separated unambiguously in this system. It is likely that the solvent-solute interactions control the (17) J. 0 . Edwards and R. G. Pearson, J . A m . Chenz. Soc., 84, 16 (1962).
nucleophilicities observed. For example, thiocyanate ion, which is more basic and more polarizable than the halide ions, should be an effective nucleophile. The lack of reactivity of thiocyanate must be due to its considerable stability in both protic and aprotic solvents. Thus, the nature of the solvent is critical in understanding reactivity in the system investigated in this paper and, in general, should be taken into account whenever comparisons of nucleophilicity are made among solvents of different types. Acknowledgment.-This work was supported by the Sational Science Foundation under Grant No. GP296%.
COSTRIBUTION FROM THE DIVISIOXOF CHEMISTRY, XRGONNE XATIONAL LABORATORY, ARGONSE, ILLINOIS
Substoichiometry of Tungsten Trioxide ; the Crystal Systems of W03.00,WO,.,,, and W02.96 1 BY ELIZABETH GEBERT A N D R. J. ACKERMAXX
Received June 2 , 1965 From the results of powder and single crystal X-ray measurements together with measured densities and chemical analyses i t has been demonstrated that substoichiometric tungsten trioxides possess structures which are significantly different from that of the stoichiometric trioxide. For the composition WOz.g8 the space group is P21/m and the unit cell contains four tungsten atoms and has the dimensions a = 7.354 41 0.005 A,, b = 7.569 +C 0.005 A,, c = 3.864 i 0.005 A,, and p = 90.6". The tungsten subcell is of the same type but slightly larger than that of the stoichiometric oxide. The results for the c o n ) the space group P2/c and a unit cell containing the formula W 5 0 0 ~and 4 s having the cell constants position W 0 2 . 9 6 ( ~indicate a = 11.90 i 0.02 A,, b = 3.826 4~ 0.012 A,, c = 59.64 i. 0.06 A,, and p = 98.4'. The proposed structure is uniquely solved for the x and z coordinates but not for the y coordinates, which appear to be located in a number of plaues staggered about y = '/z. Each unit cell contains two hexagonally-shaped ordcred defccts that are bisected by recurrent dislocation planes. A higher temp'erature polymorph, W O Z . ~ ~ ( with P ) , a unit cell tentatively containing the formula %'usO:i becomes stable at approximately 1250".
Introduction The basic chemical and physical properties of binary compounds of the group V I transition metals Cr, N o , and W are generally complex. In recent years, a number of investigations dealing with the crystallographic and thermodynamic behavior, particularly of Mo and W oxides, have elucidated the complex chemical bonding that occurs both in the solid and vapor phases. Furthermore, in the case of a number of transition metal oxides, carbides, sulfides, and phosphides, gross deviations from ideal stoichiometry are readily obtained and must be acknowledged in physicochemical descriptions of these systems. In a recent thermodynamic investigation of the tungsten-oxygen system2 it was observed a t temperatures of 13001550OK. that tungsten trioxide becomes substoichiometric and evaporates congruently a t a composition near WO2.96 under the influence of the particular vacuum conditions (10-G-10-7 mm. pressure) employed. (1) Based on work peifotmed under the auspices of t h e U S Atomic Energy Commission. ( 2 ) R.J. Ackermann a n d E G l i a u h , J . Phys. Cheirz , 67, 2696 (1963).
The X-ray diffraction patterns of powders of this material at room temperature are significantly different from those of the stoichiometric trioxide and cannot be explained on the basis of only an oxygendeficient trioxide structure. Actually, the existence of a substoichiometric region of WOa was first suggested by Glemser and S a ~ e r who , ~ reported that the basic structure of the WO3 phase extends to the composition W02.9b. However, Hagg and Magneli4refer to a paper given by Westgrenj in which is proposed the existence of a new oxide phase corresponding to approximately W 0 2 . 9 7 . GadoGhas recently reported the existence of a. phase between W200jsand WOs. The structure a t room temperature of the unit cell of the stoichiometric trioxide as reported by Andersson7 and by previous investigators contains four K O 3units and has the space group P21/a; however, the direct observations by ( 3 ) 0. Glemser and H. Sauer, Z . aizoi'g. C h e m . , 262, 144 (1043). (4) G. Hagg and A . hlagneli, A ~ k hK e m i , . l f i n e T a l , Gcol., 19A, KO,2 (1944). (6) A. Westgren, S o ~ d A'atwjoi~skarmble! . Helsingfors, 89 (1936). (6) P. Gado, Acia clys:., 16, P a r t 13, A182 (1963). (7) G. Bndersson, Acia Cheiiz. Scmzd., 7, 154 (1933).
Vol, 5, No. 1, January 1966 TanisakP of weak first- and third-order layer lines on rotation photographs, taken with the c axis rotating, indicate a unit cell containing eight WOOunits with a P21/n space group and a c axis which is twice that of hndersson's. Since there appear to be a number of divergent conclusions dealing with the trioxide and its region of substoichiometry the present investigation was undertaken in an attempt to contribute to a greater understanding by means of a further analysis of this rather complicated system. In the present investigation the conclusions are to be drawn from both powder and single crystal diffraction data and measured densities obtained a t room temperature and chemical analyses. Experimental Section The samples of tungsten oxides corresponding to the range of composition WOa-W02.86used in this investigation were prepared vza two methods. In the first, the composition WOz.96 resulted from the reduction of stoichiometric trioxide in the interval of 1050-1225" under vacuum and in the second the reaction of the appropriate amounts of trioxide and metal powders a t 1250-1300" under a purified argon atmosphere produced apparently homogeneops products of the desired composition. In the former method the samples employed were the actual residues (O/W = 2.963) of the effusion measurements described by Ackermann and Rauh .z The samples produced after several mm.) possessed a deep, dark hours of heating 2% vacuo (-lo-' blue color and contained fine, dark needles which appeared to be well-defined single crystals. However, the degree of crystalline size and homogeneity of these residues appeared to be somewhat unsatisfactory because of the relatively poor definition of high angle reflections in the powder patterns. Additional heating for about 1 hr. under vacuum a t approximately 1050' generally enhanced the definition of these reflections. It was impractical to heat for longer periods of time in order to obtain larger crystals because of the great extent of free evaporation of the samples i l z wacz~oa t the temperatures involved. In order to prepare samples a t higher temperatures, it was necessary to employ an argon atmosphere or sealed platinum capsules to reduce the rate of evaporation of the sample and thereby allow considerably longer periods of heating. Samples (-10 9.) of desired composition were synthesized by intimately mixing appropriate weights of tungsten and tungsten trioxide powders and allowing these to react a t 1250-1300° in a platinum tube containing an argon atmosphere that was initially purified of water vapor and oxygen by means of columns of magnesium perchlorate and hot copper chips, respectively. The use of platinum as an inert container has been previously demonstrated.z Before the introduction of the sample, the platinum tube was outgassed in vacuo a t 1300". In spite of these precautions, oxidation of the top portion of some of the sample occurred. The lower portions of the samples were subsequently analyzed by the combustion of a weighed sample (2 to 3 9.) in air a t 800' until constant weight was achieved and the light yellow-green color of the stoichiometric trioxide was obtained. The reproducibility of this method of preparation and analysis was generally sufficient to establish the atom ratio within h0.005. Samples having the composition O/W = 2.960 i 0.005 that were heated for periods of 2 days, 2 weeks, and 6 weeks yielded identical powder patterns that showed excellent definition a t high diffraction angles. Progressively larger crystals resulted with the increase in time of heating and the crystals obtained in this manner were in general twinned about the axis of rotation. However, distinct differences in the powder patterns were noted when a comparison was made with the patterns of the fine needles obtained in the residues of the vacuum reduction of WOS. The samples resulting from both methods of preparation had the typical slippery "graphite-like" quality upon grinding ( 8 ) S. Tanisaki, J . I'hys. SOL.J a p u n , 18,873 (1960)
SUBSTOICHIOMETRY OF TUNGSTEN TRIOXIDE137 which is usually characteristic of a layer-type structure. In the course of the syntheses of samples, O/W = 2.99, 2.98, 2.97, and 2.96, it was apparent that as the atom ratio is decreased from 3.00 the color of the sample evolved through blue-green to a deep blue a t O/W = 2.96. The densities of samples of various compositions were measured by a pycnometric method. In order to minimize the effect of trapped gases in isolated voids in the finely powdered samples which causes the incomplete filling of the pycnometer by the immersing fluid and, hence, leads to low values of the density, the following precautions were taken. The samples (approximately 2 9.) were loaded into the pycnometer (2 ml.) which was then evacuated slowly in a modified vacuum desiccator. The immersing fluid, namely water t o which was added a small amount of aerosol to decrease its surface tension but not affecting its density, was then added to the sample under vacuum by means of a separatory funnel attached to the desiccator through a rubber stopper. After the sample was completely immersed, it was gently boiled under vacuum by means of a heat lamp, then removed from the desiccator and centrifuged in order to precipitate any small particles suspended in the meniscus. The remaining operations including the weighings were done in the conventional manner. All weighings were performed after the pycnometer and contents had been equilibrated to 24-25'.
Determination of Lattice Parameters and Structures Powder Measurements.-A comparison of the low angle diffraction lines of samples of stoichiometric and substoichiometric tungsten trioxide obtained with copper K a radiation is made in Table I. A close correspondence in both d values and intensities for the reduction of WOOto WO2.98 indicates that the tungsten atoms retain essentially the same relative positions, although for the latter composition the d values are considerably larger, indicating an enlargement of the unit cell with respect to the subcell of WOs based on the structure by Tanisaki8 Similar measurements of a sample W02.99 yielded d spacings that were between those of WOa and W02.g2.. Hence, the tungsten subcell is of the same type in the WO3-WO2.98 region. One immediately sees that the diffraction patterns for materials of composition WOz. 96 are vastly more detailed than those of WOO and W02.98. Since the films of WOz.g6 showed more clearly the greater complexity of the powder patterns, film measurements of this composition are reported in Table I. The sample of W 0 2 . g 6 ( ~ ) is one of the actual residues of the vapor pressures measurements of Ackermann and Rauh, which was produced b y heating initially stoichiometric trioxide in vucuo a t 1050-1225°. The material W02.96(P)resulted from direct synthesis of tungsten and tungsten trioxide powders a t 1250-1300" under an argon atmosphere followed by rapid quenching. The W02.9e(P)pattern can be readily distinguished from that of W 0 2 , 9 6 ( ~ ) by the prominent line which is located between two strong lines a t d = 3.760 in the former compared with the faint line a t d = 3.71 in the latter, by the closer packing of the two prominent lines in the region of d = 2.65, and by the intensity differences and the lesser number of lines in the region of d = 1.94-1.80. I n general the powder patterns of WOz.9 6 ( P ) had fewer and better defined reflections. The conversion of the B to the CY phase was accomplished by heating in vucuo a t about 1100' for several
Inovgunic Chemistry positions of the tungsten atoms, that occur in the relatively narrow composition range between WOa and WOS.96.
IL d ( f . $
1.827 vwu 3.49
3.784 VvYw 1.76
vvvw 3.33 YYYW
vw 1.679 M
1.676 VINW 2.91
2.693 w 1.47 w 2.50
vvvw 1.36 Y
Single Crystal Measurements. (1) W03.00.-Single crystal photographs taken of stoichiometric trioxide confirmed the necessity of doubling A4ndersson's value7 of the c axis as recently reported by TanisakL8 The values of the monoclinic parameters agree (see Table 117) within experimental error with those reported by Tanisaki, from which parameters one calculates a theoretical density of 7.294 g./cm.3. The density measured pycnometrically in this investigation is 7.286 g./cm3. (2) WOn.gs.-The substoichiometric trioxide having the composition WO2.98 was composed of dark bluegreen crystals that were semitransparent plates or short cylinders. These crystals did not have the graphite-like quality when ground that was very noticeable in the case of the materials. Single crystal photographs showed a monoclinic cell belonging to the space group P21/m. The Weissenberg photographs of the various layers were quite similar to those obtained for TVO3.0~ although there mas no indication of the doubling of the c axis as observed for the stoichiometric trioxide. By assigning equal weight to each reflection in a least-squares treatment of diffractometer measurements of a powder sample, one obtains the cell parameters: u = 7.354 f 0.0051~k., b = 7.569 h 0.005k,c = 3.854 0.005 and p G 90.6". These parameters correspond to a unit cell containing four tungsten atoms and a calculated density of 7.17.1. g . / ~ m . which ~, compares favorably with a measured density of 7.162 g./cm. 3. In two samples having over-all compositions W02.981and W02.983there were a number of black needle crystals that proved to be the WO2. 96 structural type although the powder patterns taken of these samples failed to show the presence of this additional phase because of its low concentration. .-The preliminary study of powder (3) W02.96(a:) samples had shown significant differences in both intensities and diffraction angles from the W03-type subcell which are indicative of a basic change in structure. The further elucidation of these structural differences was accomplished by measurements of single crystals obtained from the evaporation residues of a previous investigation. Some of these crystals were unsatisfactory because they gave rise to streaking of the reciprocal lattice points. Equi-inclination Weissenberg photographs were taken of a needle having the dimensions 0.005 X 0.017 X 0.404mm.,with Cu Ka:radiation using the multiple film technique. Using the lines of copper powder as an internal standard the following cell dimensions were obtained from rotation and Weissenbergfilrns: a = 11.90 f 0.02,&., b = 3.826 0.012A., c = 59.64 It 0.06A., p = 98.4", a: = y = 90". The measured density of 7.126 g . / ~ m and . ~ the determination of the chemical composition O/W = 2.96 indicates the presence of 50 tungsten and 148 oxygen atoms in the unit cell. The theoretical density is 7.144 g./
SUBSTOICHIOMETRY OF TUNGSTEN TRIOXIDE139
Vol. 5, No. 1, January 1966
Figure 1 . 4 1 0 projection of the proposed structure of W02.9e(~).
Weak reflections on the hll and h21 layers were observed when 1 = 2n 1, which requires that the y coordinate cannot be 0 or I/%. The systematic absence of h01 reflections when 1 = 2n 1 indicated the space groups P2/c-C2h4 and Pc-CS2. The mean value of the experimentally-derived normalized structure factor, E = 0.75, compared with theoretical values of 0.798 and 0.886 for centric and acentric space groups, respectively, indicates that the centric P2/c is the preferred one. When a single crystal was rotated about the b axis, the layer-line films showed sequences of reflections lying on the reciprocal net centering about the locations of reflections for a corresponding layer-line film of WOs.00. There was a gradual loss of intensity as the distance from the location of the corresponding WOa.oo reflection increased. The intensity relationships on the hll and h21 layers generally paralleled those of the hOl’s. The intensities were measured by visual comparison with an intensity strip. The intensities were corrected for Lorentz polarization and scaled by the data reduction program of N ~ r m e n t . A ~ Patterson projection of ,401 was made using the Sly-Shoemaker Fourier program.1° Placing the tungsten atoms in locations suggested by the Patterson projection corresponding to 2(b) and 4(g) of P2/c, calculation of the structure factor was made with the Busing-Levy least-squares program.11z12 Arbitrary weights of 5 , 4.5, and 4 for
(9) H . G. Norment, “An X - R a y Diffraction D a t a Reduction Program for t h e I B M 704 and 7090,’’ Naval Research Laboratory Report 5739, Feb. 16, 1962. (10) W. G. Sly and D. P. Shoemaker, “ M I F R I , Two- and Three-Dimensional Crystallographic Fourier Summation Program for t h e IBM-704 Computer,” Massachusetts I n s t i t u t e of Technology, Department of Chemistry Technical Report, July 1, 1960. (11) W. R . Busing and H. A. Levy, “A Crystallographic Least-Squares Refinement Program f o r thc I B M 704,” Oak Ridge National Laboratory, Central Files No. 59-4-37, April 14, 1960. (12) W. R. Busing, K . 0. Martin, and H. A, Levy, “OR FLS, A Fortran Crystallographic Least-Squares Program,” Oak Ridge National Laboratory Report, OliNL-TM-305, Nov. 21, 1962.
strong, weak, and unobserved reflections, respectively, were assigned to the values of Fa. The reliability factor
was obtained for the h01 layer. A three-dimensional Patterson synthesis indicated that y = 0 or ‘/z which is impossible since hkl reflections occurred when 1 # 2n. A Patterson projection of Okl data, badly affected by absorption and limited in number, indicated that all the y coordinates are not in equivalent positions, ie., do not form two planes of tungsten atoms. When the y’s were inserted a t various sets of locations in either 4(g) of P2/c or 2(a) of Pc an over-all minimum value of R N 0.28 was obtained for all observed reflections from a least-squares treatment. However, the final y coordinates were not unique. The h21 layer often had an R factor approximately twice that obtained for the h l l layer. Difference Fouriers of observed reflections and difference Fouriers containing unobserved reflections which had been calculated as I m i n / 3 as suggested by Hamiltonla mere of no aid in uniquely locating the y coordinates. Although i t was impossible to establish the y coordinates, it is suggested that they could be located in a number of planes staggered about y = l / 2 . An alternative is the existence of microphases or regions within the crystal having different types of alignment of the staggered tungsten layers. Weak satellite reflections surrounding the most intense reflections in the Weissenberg photographs and the high R factor for the h01 layer indicate that there also may be significant misalignments among the domains within the single crystal even in the x-z plane. The 010 projection of one-half the unit cell of the proposed ordered-defect structure is shown in (13) W. C. Hamilton, Acla Cvyst., 8 , 185 (1955).
TABLE I1 OBSERVED ASD CALCULATED STRUCTURE FACTORS FOR W j ~ O l a ~ i
L F C B S I F C A L I FUBS F G B S
L F O B S I F C A L l FG8S P U B 5
L F U B b IFChLI F O U i F O U S
L i-iiii I F i A L I F O U S F O B S
L FOBS IFCALI FOBS FCBS
L F O H S I F C A L / F O U 5 FUAS
a The first and second columns of structure factor values contain F, and ' F,:for h0Z; the third and fourth columns contain F , for h l l and h21, respectively.
TABLE I11 TUNGSTEX POSITIOSS IS THE UXITCELLWjoOlia Positionsa
2 in 2(b) 4 in 4(g) 4 in 4(g)
0.5 0.127 0.374 0.060 0.371 0,429
0.0 3'1 0.037 32 0.299 4 in 4 ( g ) Y3 0.101 4 in 4( g) ?4 0.118 4 in 4(g) ?: 0.061 4 in 4(g) 0.064 y6 0.276 Yi 0,341 4 in 4(g) 0.003 4 in 4(g) 0.186 ?s 0.476 4 in 4(g) 0.268 Ys 0.245 4 in 4(g) 0.310 3i n 0.184 4 in 4(g) 0.239 3.11 0.420 4 in 4(g) 0.309 YlZ 0,356 a If the true space group is Pc, then the y coordinate in 2( b ) is undetermined and 4(g) becomes 2(a) with another set of 12 positions a t 2 j i # corresponding to those given for 4(g).
Figure 1. Observed and calculated values of the structure factor for izOl reflections and observed values for the hlZ and h2Z are given in Table 11. A value of 0.12 was used for an over-all, isotropic temperature factor. The x and z coordinates of the 50 tungsten atoms in the unit cell are given in Table 111. (4) W 0 2 . ~ ( $.-The ) single crystal measurements and structure determination of this phase are not coinplete a t the present time; however, a discussion of some of the preliminary findings seems quite pertinent. Microscopic examination of this polycrystalline material showed that many of the smaller needles were bent
and the crystallite size was generally larger than previously obtained for WO,.~G(C~). The larger crystals were due to the longer period of heating a t a rclativcly higher temperature. Initially all of the crystals selected for single crystal measurements were twinned. Ultimately a single crystal was selected from a sample that had been heated G weeks a t approximately 1250" under an argon atmosphere. A powder photograph of a sample of this material proved to be that of the W 0 2 . y 6 (@)phase shown in Table I. The b axis rotation photographs of the crystal appeared to be similar to that of \VO2.9~(a). The Weissenberg photographs were very similar to those of W O ~ . ~ G although (C~) visual inspection revealed a more rapid decrease in intensity for hkl reflections when 1 = 2n. When 1 # 27a the reflections were absent, indicating y = which is contrary to the findings for the 7V02.96(o()crystals. This observation would appear to confirm the previous observation that the W O Z . ~ G (isP )a more symmetrical version of W02.9~(a) because the former was found to be a higher temperature polymorph of the latter. These preliminary findings suggest that the G axis is half the length of the c axis in W02.96(a)and the space group is P2/m. The xz projection of the unit cell containing the formula W2507si is very likely that in Figure 1 with the tungsten atoms lying in a plane with the origin a t
As was previously mentioned crystals of the W 0 2 . 8 6 structural type were present in samples of W02.9ul
SUBSTOICHIOMETRY OF TUNGSTEN TRIOXIDE141
Vol. 5, No. 1, January 1966
TABLE IV COMPARISON OF CRYSTALLOGRAPHIC PARAMETERS OF TUNGSTEN OXIDES Chemical compn.
Formula of unit cell
a , A.
b , A.
g. c m . 7
7.68 90.9O 7.294 7.286 8 7.53 7.30 3.854 90.6" 7.169 7.162 This study 7.569 7.354 3.826 59.64 98.4" 7.144 7.126 This study W60Ol48 11.90 -3.826 ~29.82 -98.4' This study -11.90 Wz6074 23.59 95.72' 7.163 7.15 b 3.767 WzoO5s 12.05 wo2.90 13.98 115.14' 7.781 7.958" C 3.775 Wi8049 18.28 W0z.n 5.550 120.42 10.82 ... d 4.892 We08 5.650 woz A. Maga Measured in this investigation for a sample having the composition W 0 ~ . 7 ~ 7 . A. Magneli, Arkiv. Kemi, 1, 513 (1949). A. Magneli, Arkiv Kemi, Mineral. Geol., 24A,No. 2 (1946). neli, ibid,,1,223 (1949).
Wos WOZ.98 WoZ.s€.(CU) WOz.ge(P)
and WO2. 988 which were prepared a t approximately 1250". Weissenberg photographs of several of these crystals indicated intensities for hkl reflections for 1 = 2n that were only slightly different from w02.96((r)and cell dimensions that appeared to be the same within the precision of measurement. The intensities were noticeably much weaker for hkl reflections when 1 # 2n, which indicates a greater ordering of the tungsten planes with the y coordinate nearer '/z than in W02.96 (01). Hence, the degree of staggering of the tungsten atoms about y = ' / z for these crystals appears to be between that of Woz.g6(0() and W02.96(@)and suggests that the mechanism of the [email protected]
phase transition may involve successive stages of unpuckering of the tungsten planes.
Discussion There are several interesting features of the proposed structure of W02.96(a) which can be seen by reference to Figure 1. Each unit cell in the projected plane contains two ordered defects having the shape of a distorted hexagon. These defects are bisected by a recurrent dislocation plane shown by the dotted line. The W-W distance across this plane is considerably shorter than those elsewhere in the structure and, hence, there are probably no oxygen atoms interleaved between the tungsten atoms in this plane. It is assumed that the tungsten atoms not in this plane are surrounded by a distorted octahedron of oxygen atoms. In these aspects the structure is similar to those of other tungsten and molybdenum oxides.14 However, based on the number of tungsten atoms found in the unit cell and the number of oxygen atoms required by the composition W02.g6,it is necessary to insert oxygen atoms a t x _N l/%, y 3+1 0,z 'v '/4, "4. The presence of these atoms requires that two of the tungsten atoms in the region of the defect be coordinated with seven oxygen atoms, probably forming pentagonal bipyramids as pointed out by KihlborgI5 for other molybdenum and tungsten oxides. The three-dimensional defect channels, therefore, cannot be open holes as in the case of W20058and other known structures.16 The Weissenberg films were extremely difficult to measure not only because of the inherent difficulties in a large unit cell but also because of the large areas of no reflections on the reciprocal lattice. Of a possible 4080 (14) A. Magneli, Acta C y y s t . , 6,495 (1953). (15) L.Kihlborg, Arkiw Kemi, 21, 471 (1963).
reflections only 903 were observed. Furthermore, surrounding the most intense reflections were weak satellite reflections which are indications of crystal imperfection and disorder. The presence of this disorder is an additional factor which permits only a tworather than three-dimensional solution of the crystal structure. A method of preparation of more perfect crystals a t somewhat lower temperatures is believed necessary for any future study. The results of the diffractometer measurements indicate that the trioxide phase can become substoichiometric down to W02.98. The single crystal measurements, however, indicate some subtle variations with composition change. The unit cell of WOn.ssa t room temperature is slightly larger than the corresponding tungsten subcell of stoichiometric WOs. I n the latter case the results of Tanisak? confirmed in this study indicate two kinds of WO6 octahedra. When oxygen is randomly removed from this structure to form W02.98 these two octahedra appear to become indistinguishable. Certain features of the high-temperature phase diagram based on vaporization phenomena proposed b y Ackermann and Rauh2 can now be further clarified. Since there exist quite pronounced differences in the structures of W02.96 and W02.98, and since powder patterns of the composition WOZ. 97 quenched from 1200' appear to be a two-phase mixture, a miscibility gap probably extends up to a t least this temperature. There also appears to be a correlation between the incongruent evaporation of the composition W02.96 a t temperatures above approximately 1250O and the a to p phase transformation which occurs in the same region of temperature. The higher symmetry of the tungsten planes in the /3 phase is very likely a manifestation of a decrease in the strength of the W-0 bond which permits the preferential loss of oxygen and the formation of the W2~,Osgphase in which the tungsten planes are completely unpuckered. l4 A comparison of the crystallographic parameters of presently known tungsten oxides is presented in Table IV. Close agreement between the calculated and measured values of the density is seen in all cases except those for W&9. The crystal density passes through a distinct minimum for the W60014sphase in disagreement with earlier work reported by Glemser and Sauer3 which shows a gradual increase from WOs to WOZ. The earlier work, however, must be viewed with some reservation because the value reported for a mix-
142 R. WANG,H. STEIKFINK, AND W. F. BRADLEY
ture of W p 0 0 and ~ Wl8Oeg (over-all composition W 0 2 . g 2 ) is significantly greater than the values reported for each of the nearly pure phases. The existence of additional defect structures prepared under different conditions and having compositions differing only slightly from that of UT02.9e remains a distinct possibility. The recent observations by Gado6b16 indicate a structure which is quite different from that (16) P. Gado, Research Institute for Telecomm. Techn., Budapest, Hungary, private communication.
proposed here, and the observations by Kellett and Rogers" may indicate a new phase which is different from those previously observed. Acknowledgments.-The authors wish to acknowledge Mr. James H. Maurer for assistance in the preparation of samples and Dr. Stanley Siege1 for useful criticism and discussion throughout the courqe of thi.; investigation. (17) E A Kellett and S E Rogets, J C Z ~ c l ~ o c h r Soc m 110, 502 (196'3)
DEPARTMEKT OF CHEMICAL ENGISEERING, TJNIVERSITY OF TEXAS, AUSTIN,TEXAS
The Crystal Structure of Lanthanum Telluride and Tellurium-Deficient Neodymium Telluride' BY R. WAXG, H. S T E I S F I S K ,
W. F. BRADLEY
Recehed July 12, 1965 Single cryqtal X-ray diffraction studies of LaTeZ and lTdTezand of the related tellurium-deficient compositions have confirmed the isomorphism with Fe& ( C 38). Two different types of tellurium atoms exist in the structure. The atoms in the basal plane are essentially metallic in nature and give rise t o the observed electrical properties. These are the atoms which can be removed from the structurc t o produce the tellurium-deficient compositions. This explains the increased electrical resistivity as well as the decrease in the length of the n axis and the increase in the length of the c axis observed for these compounds
Introduction The crystal structure of LaTe2 was reported as isostructural with CeTep by Pardo, Flahaut, and Dom a ~ ~ g e and , ~ , ~both compounds appear to be isostructural with the Fe2As structure, C 3SL4 Since lanthanum and cerium have atomic numbers which are close to the atomic number of tellurium, the differences in atomic scattering factors, especially after applying a dispersion correction, are small enough to prevent the unequivocal assignment of locations for these atoms. The previous structure investigations were based on data derived from powder patterns. Investigation of the structures of the two isomorphs PJdTe2 and LaTet by means of single crystal techniques promises to locate definitely the atomic species. The neodymium compound, with the greater scattering factor difference, was also deficient in tellurium. It afforded a firm distribution of the atomic species among alternative equivalent position sets, which could then be applied to the LaTez. Experimental Section Lanthanum and neodymium were treated with tellurium by a vapor-solid reaction in sealed Vycor tubing a t 600" to yield com(1) Research sponsored b y t h e Air Force Office of Scientific Research, Office of Aerospace Research, United States Air Force, under AFOSR Grant No. 806-65. (2) M. P. Pardo, J . Flahaut, a n d L. Domange, C o m p t . r e n d . , 206, 953
(1963) (3) A I . P. Pardo, J. Flahaut, and I,. Domange, Bull. soc. chim. Fvnncr, 3267 (1964). (4) A. F. Wells, Structural Inorganic Chemistry, 3rd Ed., Oxforrl TJniversity Press, T.ondon, 1961, p. 520.
pounds having formulas LaTez o and NdTe18. The space group for these compounds is P4/,nim, and the unit cell constants obtained from powder data are a = 4.507 + 0.005 .k., c = 9.128 i 0.010 A. for LaTez o and a = 4.377 + 0.006 .k., c = 9.060 0.010 d . for NdTel there are 2 formula weights per unit cell. The room temperature variation of lattice constants c, a, and c / a as a function of composition for the iXdTez-. solid solution range has been reported by Lin, Steinfink, and Weiss.6 Single crystals of LaTe2 0 of dimensions 0.07 X 0.06 X 0.007 mm. and of the approximate composition r\-dTel of dimensions 0.05 X 0.04 X 0.01 mm. were mounted along the c axis. The three-dimensional intensity data from both crystals were collected with a G.E. XRD-6 single crystal oricnter using Cu Ka radiation and a scintillation counter with pulse height discrimination. Absorption corrections were necessary because of the high linear absorption coefficients of LaTe2 and NdTez, 2126.7 and 2370.5 ern.-', respectively. The shapes of the somewhat irregular fragments were approximated by a small number of boundary planes, and the absorption corrections were computed by the Busing and Levy method.B This shape approximation of the fragment was rather idea1iLed for the two large dimensions, making the hkO reflections subject to large absorption errors. In this structure the 2 and y parameters are fixed by symmetry so the hkO reflections were omitted from the refinement calculations. The scattering factors of La, Nd, and T e were corrected for dispersion, isotropic as well as anisotropic temperature factors were used, and a full-matrix, least-squares refinement with unit weights was carried out based on the FezAs model.
Structure Determination Table I shows the final positional parameters and the anisotropic temperature factors together with their ( 5 ) W. Lin, H. Steinfink, and E. J. Weiss, Inovg. Chrm., 4 , S i 7 (1065). ( 6 ) W.R. Busing and H. A. Levy, Acla C ~ y s t . 10, , 180 (1957).